# Representative volume element to estimate buckling behavior of graphene/polymer nanocomposite

- Avinash Parashar
^{1}and - Pierre Mertiny
^{1}Email author

**7**:515

**DOI: **10.1186/1556-276X-7-515

© Parashar and Mertiny; licensee Springer. 2012

**Received: **26 June 2012

**Accepted: **4 August 2012

**Published: **20 September 2012

## Abstract

The aim of the research article is to develop a representative volume element using finite elements to study the buckling stability of graphene/polymer nanocomposites. Research work exploring the full potential of graphene as filler for nanocomposites is limited in part due to the complex processes associated with the mixing of graphene in polymer. To overcome some of these issues, a multiscale modeling technique has been proposed in this numerical work. Graphene was herein modeled in the atomistic scale, whereas the polymer deformation was analyzed as a continuum. Separate representative volume element models were developed for investigating buckling in neat polymer and graphene/polymer nanocomposites. Significant improvements in buckling strength were observed under applied compressive loading when compared with the buckling stability of neat polymer.

### Keywords

Multiscale model Nanocomposite Buckling Finite element method## Background

In the recent past, graphene has emerged as a potential candidate for developing nanocomposites with improved properties [1, 2]. The experimental characterization of graphene/polymer nanocomposites is a challenging process, and hence, computational approaches for predicting the behavior of such materials have also extensively been employed. Various multiscale models are available in the literature for predicting the properties of carbon nanotube (CNT)-based nanocomposites [3–5], but very few models have been presented to study graphene nanocomposites. For example, Cho et al. [6] developed a numerical model in conjunction with Mori-Tanaka approach to study the elastic constants of randomly distributed graphene in polymer. Awasthi and his team [7] investigated the load transfer mechanism between polyethylene and graphene sheets. Montazeri and Tabar [8] developed a finite element (FE)-based multiscale model to investigate the elastic constants of graphene-based nanocomposites.

Buckling in isolated graphene sheets was modeled by several researchers [9–11]. However, buckling stability of graphene/polymer nanocomposites was only reported by Rafiee et al. [12]. Using an experimental and analytical approach, up to 50% and 32% improvement in the buckling stability of nanocomposites was reported respectively. In the analytical approach, an Euler buckling formulation was employed, and elastic properties required in the Euler equation were estimated by experimental means. The discrepancies between the two buckling stabilities were attributed to scaling issues.

It is well established that the reinforcement of polymer with graphene increases the elastic modulus of the material which further improves buckling stability. The aim of this study is to propose a numerical model which can estimate the increase in buckling stability with different volume fractions of graphene and can further be extended to complex shapes and structures.

It has been reported that achieving a uniform dispersion of two-dimensional graphene sheets in polymer is more challenging compared to the mixing of one-dimensional CNT. Moreover, the application of nanocomposites is not limited to simple structures, and the comprehension of material behavior in complex structures is restricted when employing experimental and analytical methods. Consequently, research efforts are increasingly focused on numerical approaches. To overcome some of the limitations that exist in experimental and analytical work, a multiscale representative volume element (RVE) is proposed in this paper to investigate buckling phenomena in graphene/polymer nanocomposites under the assumption that graphene is uniformly distributed in the polymer. To the knowledge of the present authors, no numerical model has been reported yet to study the effect of graphene on the buckling strength of nanocomposites. In the proposed technique, graphene was modeled in the atomistic scale, whereas polymer deformation was analyzed as a continuum.

## Methods

### Finite element modeling of RVE

In this paper a finite element technique was employed in conjunction with molecular and continuum mechanics to simulate buckling in graphene/polymer nanocomposites. In the proposed RVE, the polymer, epoxy in this case, was modeled as a continuum phase whereas the deformation in graphene was evaluated using an atomistic description. Nonbonded interactions were considered as the load transfer mechanism or interphase between polymer and graphene. FE modeling was performed in the ANSYS (Version 13) software environment (ANSYS Inc., Canonsburg, PA, USA).

#### Atomistic model for graphene

*V*

_{bonded}represents the bonded interaction between atoms and is considered primarily responsible for maintaining the structural integrity. The potential energy term ‘

*V*

_{nonbonded}’ includes electrostatic forces, e.g., van der Waals forces, which are considered weak in nature and can generally be neglected in comparison to bonded interactions. Li and Chou [13] established a correlation between interatomic molecular potential energies and corresponding strain energies of a beam element as described by Equations 2, 3, and 4.

where *K*_{
r
} (938 kcalmol^{−1}Å^{−2}), *K*_{
θ
} (126 kcalmol^{−1}rad^{−2}), and *K*_{
τ
} (40 kcalmol^{−1}rad^{−2}) are the bond stretching, bond bending, and bond torsional resistance force constants. *E* represents the Young's modulus; *A*, the cross sectional area; *I*, the moment of inertia; *G*, the shear modulus; *J*, the polar moment of inertia of the beam element, respectively. BEAM4 elements were used in the ANSYS software environment to model graphene by connecting nodes, and material properties for those elements were estimated with the help of Equations 2, 3, and 4.

#### Continuum model for polymer

The volume fraction of graphene in polymer ranges commonly up to 10%. Most of the material volume is therefore occupied by polymer. Simulating the polymer phase on the atomistic scale would require large efforts in dealing with large numbers of degrees of freedom as well as substantial computational cost. Therefore, as a reasonable compromise, the polymer phase was modeled as a continuum, and three-dimensional SOLID45 elements were used for meshing the geometry. Epoxy with a Young's modulus of 3.4 GPa and a Poisson’s ratio of 0.42 was considered as the polymer material in the present work.

#### Interphase between graphene and polymer

*r*is the atomistic distance between atoms,

*φ*(0.34 nm) is the hard sphere radius, and

*γ*(0.556 kcal/mole) is the potential well depth. In the finite element environment, these nonbonding interactions were modeled with the help of LINK8 truss elements. As shown in Equation 6, properties for those truss elements were estimated by comparing the classical continuum strain energy of truss elements with the Lennard Jones ‘6-12’ potential. Note that the truss model described herein was earlier employed by Li and Chou [14] to simulate the interaction between CNT and epoxy polymer.

*R*

_{Eq}is the initial undeformed length,

*r*is the deformed length,

*A*is the cross sectional area, and

*E*(

*r*) is the Young's modulus of the truss element.

#### Eigenvalue buckling analysis

A linear analysis for mode one buckling was performed in this work, which is associated with the computation of a bifurcation load and corresponding buckling mode. The analysis in the finite element environment was divided into two sections, i.e., a pre-buckling and a post-buckling analysis [15].

#### Pre-buckling analysis

*S** within each element. These computed reference values are then used for estimating the geometric stiffness matrix

*K*

_{ G }, which is needed in the post-buckling analysis. To initiate the analysis in the finite element model, the general matrix form equation provided in Equation 7 was employed to estimate nodal displacements [

*Q*] when the structure is subjected to the reference unit load

*P*

_{ R }. In Equation 7 the total stiffness matrix [

*K*

_{ 0 }] is the assembled global stiffness matrix for the multiscale structure composed of beam, truss, and solid elements. Conventional assembly techniques can be used to obtain the global stiffness matrix.

*Q**} obtained from Equation 8 are further post-processed to compute strains and corresponding stress values

*S** within each element using Equation 9, in which matrix [

*D*] represents the elasticity matrix (material property) while matrix [

*B*] is a function of approximating polynomial or shape functions.

#### Post-buckling analysis

*λ*and

*v*are the load factor and the eigenvector of displacements. The geometric stiffness matrix

*K*

_{ G }used in Equation 10 is defined with the help of Equation 11, where Γ is composed of derivatives of shape functions and

*S*is a function of the stress

*S** estimated in the pre-buckling analysis.

*λ*

_{min}can be determined, which is then employed to estimate the buckling force given by Equation 12.

## Results and discussion

The proposed RVE was employed to understand the buckling behavior of graphene in a polymer matrix when graphene was assumed to be uniformly distributed. A second separate RVE structure with equal dimensions was developed using finite element modeling to study the buckling in neat (homogenous) polymer.

*E*) were then used in defining the homogenous rectangular plate with dimensions of the proposed RVE model. The buckling loads were calculated for this homogenous rectangular plate shown in Figure 3a and were compared with the direct approach defined in Figure 3b.

*P*

_{ x }is the applied unidirectional compressive load,

*w*is the displacement in the outward normal direction, and

*D*is flexural rigidity (i.e., a function of the Young's modulus). Boundary conditions were kept identical in all RVE models. Only the value of flexure rigidity was varied, which afforded the proposed RVE model the capability of yielding

*E*for different graphene volume fractions.

The boundary conditions along with dimensions for the proposed RVE model are shown in Figure 3. The thickness of graphene in the atomistic scale and for epoxy as a continuum phase was kept constant at 0.344 nm, whereas the thickness of the interphase was kept at 0.172 nm according to [14]. The graphene volume fraction in the proposed RVE model was varied by changing the size of the graphene sheet, leading to graphene volume fractions ranging from 2% to 6%. Filler volume fractions of reasonable and practical magnitude were thus studied, omitting the agglomeration effects in graphene nanocomposites with high filler content.

## Conclusions

In this study a representative volume element method was successfully employed to investigate the buckling phenomenon in graphene/polymer nanocomposites, where graphene was assumed to be uniformly distributed. Graphene was modeled in the atomistic scale and polymer as a continuum. A significantly enhanced buckling strength of graphene reinforced polymers was observed as compared to neat polymer, i.e., buckling strength of graphene/polymer nanocomposite improved by 26% with only 6% filler volume fraction.

## Declarations

### Acknowledgment

The authors would like to acknowledge the financial support by the Alberta Ingenuity Graduate Scholarship in Nanotechnology.

## Authors’ Affiliations

## References

- Rafiee MA, Rafiee J, Srivastave I, Wang Z, Song H, Yu ZZ, Koratkar N: Fracture and fatigue in graphene nanocomposites.
*Small*2010, 6: 179–183. 10.1002/smll.200901480View Article - Rafiee MA, Rafiee J, Wang Z, Song H, Yu ZZ, Koratkar N: Enhanced mechanical properties of nanocomposites at low graphene content.
*ACS Nano*2003, 3: 3884–3890.View Article - Ayatollahi MR, Shadlou S, Shokrieh MM: Multiscale modeling for mechanical properties of carbon nanotube reinforced nanocomposites subjected to different types of loading.
*Compos Struct*2011, 93: 2250–2259. 10.1016/j.compstruct.2011.03.013View Article - Meguid SA, Wernik JM, Cheng ZQ: Atomistic based continuum representation of the effective properties of nano-reinforced epoxies.
*Int J Solids Struct*2010, 47: 1723–1736. 10.1016/j.ijsolstr.2010.03.009View Article - Odegard GM, Gates TS, Wise KE, Park C, Siochi E: Constitutive modeling of nanotube-reinforced polymer composites.
*Compos Sci Technol*2003, 3: 1671–1687.View Article - Cho J, Luo JJ, Daniel IM: Mechanical characterization of graphite/epoxy nanocomposites by multi-scale analysis.
*Compos Sci Technol*2007, 67: 2399–2407. 10.1016/j.compscitech.2007.01.006View Article - Awasthi AP, Lagoudas DC, Hammerand DC: Modeling of graphene-polymer interfacial mechanical behavior using molecular dynamics.
*Modell Simul Mater Sci Eng*2009, 17: 31–37.View Article - Montazeri A, Tabar HR: Multiscale modeling of graphene- and nanotube-based reinforced polymer nanocomposites.
*Phys Lett A*2011, 375: 4034–4040. 10.1016/j.physleta.2011.08.073View Article - Ru CQ: Effect of Van der Waals forces on axial buckling of double-walled carbon nanotube.
*J Appl Phys*2000, 87: 7227–7231. 10.1063/1.372973View Article - Pradhan SC: Buckling of single layer graphene sheet based on nonlocal elasticity and higher order shear deformation theory.
*Phys Lett A*2009, 373: 4182–4188. 10.1016/j.physleta.2009.09.021View Article - Sakhaee-Pour A: Elastic buckling of single-layered graphene sheet.
*Comput Mater Sci*2009, 45: 266–270. 10.1016/j.commatsci.2008.09.024View Article - Rafiee MA, Rafiee J, Yu ZZ, Koratkar N: Buckling resistant graphene nanocomposites.
*Appl Phys Lett*2009, 95: 223103. 10.1063/1.3269637View Article - Li C, Chou TW: A structural mechanics approach for the analysis of carbon nanotubes.
*Int J Solids Struct*2003, 40: 2484–2499. - Li C, Chou TW: Multiscale modeling of compressive behavior of carbon nanotube/polymer composites.
*Compos Sci Technol*2006, 66: 2409–2414. 10.1016/j.compscitech.2006.01.013View Article - Waszczyszyn Z, Cichon C, Radwanska M:
*Stability of Structures by Finite Element Methods*. Amsterdam: Elsevier; 1994.

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.